Alkaline Earth Metal Ion/Dihydroxy-Terephthalate MOFs: Structural Diversity and Unusual Luminescent Properties.
Douvali, Antigoni; Papaefstathiou, Giannis S.; Gullo, Maria Pia; Barbieri, Andrea; Tsipis, Athanassios C.; Malliakas, Christos D.; Kanatzidis, Mercouri G.; Papadas, Ioannis; Armatas, Gerasimos S.; Hatzidimitriou, Antonios G.; Lazarides, Theodore; Manos, Manolis J.; Inorganic chemistry 54 (2015) 5813–5826; doi:10.1021/acs.inorgchem.5b00539

data_4343117
_publ_section_title
;
 Alkaline Earth Metal Ion/Dihydroxy-Terephthalate MOFs: Structural
 Diversity and Unusual Luminescent Properties.
;
_journal_issue                   12
_journal_name_full               'Inorganic chemistry'
_journal_page_first              5813
_journal_page_last               5826
_journal_paper_doi               10.1021/acs.inorgchem.5b00539
_journal_volume                  54
_journal_year                    2015
_chemical_formula_moiety         'C48 H66 N6 O24 Sr3, H2 O'
_chemical_formula_sum            'C48 H68 N6 O25 Sr3'
_chemical_formula_weight         1391.94
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                101.036(5)
_cell_angle_beta                 106.890(5)
_cell_angle_gamma                107.950(5)
_cell_formula_units_Z            1
_cell_length_a                   11.439(5)
_cell_length_b                   11.966(5)
_cell_length_c                   12.113(5)
_cell_measurement_reflns_used    25944
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.744
_cell_measurement_theta_min      1.881
_cell_volume                     1435.6(11)
_computing_cell_refinement       BRUKER
_computing_data_collection       BRUKER
_computing_data_reduction        BRUKER
_computing_molecular_graphics
;
 DIAMOND (Brandenburg, 2006)
 MERCURY (Bruno et al. 2002)
;
_computing_publication_material  'WINGX (Farrugia, 1999)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'BRUKER APEX'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0235
_diffrn_reflns_av_sigmaI/netI    0.0359
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            25944
_diffrn_reflns_theta_full        28.74
_diffrn_reflns_theta_max         28.74
_diffrn_reflns_theta_min         1.88
_exptl_absorpt_coefficient_mu    2.865
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.9780
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.610
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       rod
_exptl_crystal_F_000             712
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.06
_refine_diff_density_max         1.185
_refine_diff_density_min         -1.393
_refine_diff_density_rms         0.228
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.154
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     400
_refine_ls_number_reflns         7397
_refine_ls_number_restraints     16
_refine_ls_restrained_S_all      1.155
_refine_ls_R_factor_all          0.0720
_refine_ls_R_factor_gt           0.0368
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0831P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1102
_refine_ls_wR_factor_ref         0.1352
_reflns_number_gt                5513
_reflns_number_total             7397
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic5b00539_si_002.cif
_cod_data_source_block           AEMOF-5
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 3271 2015-04-21 07:52:19Z andrius 

 Adding full bibliography for 4343114--4343118.cif.
;
_cod_database_code               4343117